 Nano Express
 Open Access
 Published:
A developed expression of chemical potential for fast deformation in nanoparticle electrodes of lithiumion batteries
Nanoscale Research Letters volume 14, Article number: 262 (2019)
Abstract
In this paper, we propose a developed expression of chemical potential without the assumption of low deformation rate to account for the diffusion induced stress and the distribution of Li concentration in nanoparticle electrodes of lithiumion batteries. The difference between the developed and traditional expressions on the stress evolution in a spherical nanoparticle electrode made of silicon is analyzed under both potentiostatic and galvanostatic operations, using the derived diffusion equation and the finite deformation theory. The numerical result suggests that the difference between these two expressions of chemical potential is significant under potentiostatic operation, rather than that under galvanostatic operation. A critical radius, where there is no difference between the Li flux caused by these two expressions of chemical potential as well as the Cauchy hydrostatic stress during most of the lithiated process, is firstly reported in this work.
Introduction
For the development of portable electronic devices, electric vehicles and largescale energy storage, a number of highcapacity electrode materials such as silicon, which experience extreme changes in volume during lithiation, are proposed to be applied in lithium batteries [1,2,3]. The stressinduced by homogeneous volumetric deformation is called diffusion induced stress, which may induce brittle fracture during cyclic charge and discharge, and this negative effect further degrades the capacity of the battery [4]. Composite materials of lithiumion battery electrodes are generally complex, and their morphologies are different, which makes it more difficult to explain battery behavior by theory or equation. In theoretical models, the properties of composite materials are usually simulated by considering the changes of electrode material parameters in space coordinates, while the interface effect of composite materials is ignored. At present, three typical electrode shapes, i.e., spherical, cylindrical and plate, are mainly considered in the theoretical model. Among them, spherical and cylindrical shapes are usually onedimensional models, and both onedimensional and twodimensional models for plate electrodes are available. Recently, a number of studies have focused on the diffusioninduced stress in silicon nanoparticle electrodes of lithiumion batteries. For example, Yang et al. [5] presented a chemomechanical model to investigate the lithiationinduced phase transformation, morphological evolution, stress generation and fracture in crystalline silicon nanowires. Li et al. [6] studied the effect of local velocity on diffusioninduced stress in silicon nanoparticle electrodes. Zhao et al. [7] analyzed the diffusion induced stress with the consideration of inelastic deformation of host material. In all these aforementioned works, the fundamental physics involved is the atomic or ionic diffusion in solids under multiple driving forces. Atomic diffusion in a solid may change the solid composition from its stoichiometric state and be affected by the diffusion induced stress. Such stress and diffusion interaction is governed by the thermodynamic equilibrium of the solids.
Larche and Cahn [8] developed a thermodynamic framework for multicomponent solids which reach equilibrium under nonhydrostatic stress. The framework was based on the assumption that the deformation caused by composition change is small and isotropic. As a result, a stressdependent chemical potential was introduced to account for the interaction between stress and diffusion. Wu [9] derived a different stressdependent chemical potential in which the Eshelby momentum tensor is involved instead of the hydrostatic Cauchy stress. On this basis, Cui et al.[10] have proposed a new chemical potential for the finite deformation of solids. However, in these works, the derivation is only to be rigorous when the deformation is small or the deformation rate is low enough compared with diffusion. It is likely to make a significant error for a silicon electrode because of its large compositional volumetric expansion (∼ 400%) when it is lithiated rapidly.
In this paper, we present a developed expression of chemical potential without the assumption of low deformation rate, distinguished from the traditional expression of Cui [10]. This model is established for the fast deformation of the electrodes during charging or discharging and is independent of the morphologies because chemical potential is an intensive quantity rather than an extensive quantity. The difference between these two expressions of chemical potential on the distributions of stress and Liconcentration are analyzed under both potentiostatic and galvanostatic operations in Si nanoparticle electrodes. The result reveals that the difference increases with the increase of deformation rate. A critical radius, where there is no difference between the Li flux caused by these two expressions of chemical potential as well as the Cauchy hydrostatic stress during most of the lithiated process, is found at the same time.
Methods
Mechanical Equations
The insertion of lithium into electrodes can cause volumetric change. For convenience, we employ two ways to describe the deformation and motion of the solids, namely, the Lagrangian description and the Eulerian description. The motion of material particles in a continuum medium can be described by
where x is the Euler coordinates, X is the Lagrange coordinates, and U is the displacement field. The change in the shape of the continuum solid can be characterized by the deformation gradient tensor, given by
where Grad represents the gradient operator in the Lagrangian description, and I is the unit tensor of second order.
For a spherical particle, the Lagrange coordinates and the Euler coordinates of a material point are (R, Θ, Φ) and (r, θ, φ) respectively in the spherical system. Then, the deformation gradient tensor F is found as
During charging or discharging, the shape change of the electrode can be divided into two processes: (a) a shape change due to the insert of lithium and (b) a reversible elastic deformation. These two deformation processes can be described by two separated gradient tensors and the total deformation gradient tensor can be written as
where F^{e} represents the elastic deformation, F^{c} represents the shape change due to the insert of lithium. Equation (4) represents the process of electrode material from the initial (undeformed) state to the current (deformed) state. Assuming the shape change due to the insert of lithium is isotropic, F^{c} can be given by
where Ω represents the partial molar volume.
From Eq. (3–5), the elastic deformation gradient tensor F^{e} is
The total GreenLagrange strain tensor E can be written as
where the elastic strain tensor E^{e} and diffusioninduced strain tensor E^{c} are
respectively.
Substituting Eq. (6) into Eq. (8), the radial and tangential components of the GreenLagrange strain tensor are
The constitutive relation for the deformation can be determined from the strain energy density as
where W is the elastic strain energy density in the Lagrangian description, and P is the first PiolaKirchhoff stress. Furthermore, if the material is linearly elastic, W can be written as a quadratic function of the GreenLagrange strain tensor
Here, E_{h} and ν are Young’s modulus and Poisson’s ratio, respectively, C is the stiffness tensor, and det(F^{c}) is the determinant of the deformation gradient tensor for the diffusioninduced deformation.
Finally, the first PiolaKirchhoff stress is given by
Combining Eqs. (5), (9), (10), and (13), the corresponding components of the first PiolaKirchhoff (PK) stress tensor are
And the first PK stress must satisfy the condition of equilibrium in the absence of body force
with initial and boundary conditions
Mass Transport Equation
The concentration and the diffusion flux of lithium in electrodes, which are functions of coordinates and time, will be called C(X, t) and J(X, t) in the Lagrangian description, and they should be satisfied with the mass transport equation written as
where Div represents the divergence operator in the Lagrangian description. Considering the characteristic of spherical symmetry, diffusion occurs only in the radial direction and we use J(R, t) to represent the radial component of J(X, t). In the spherical system, Eq. (18) becomes
The diffusion of lithium in electrodes is driven by chemical potential gradient, and the radial flux J(R, t) is proportional to the gradient of chemical potential μ, as [11]
where D is the diffusivity, R_{g} is the gas constant, and T is the temperature. μ is defined as the deviation of total energy density to the concentration and can be written as
Assume that the energy density of the system, Π, can be described as the sum of chemical energy density and strain energy density. So, the total internal energy density can be written as
Substituting Eq. (22) into Eq.(21), the chemical potential μ can be shown to be
where μ_{0}(C) and τ(E^{e}, C) are the stressindependent and stressdependent parts of the chemical potential respectively. And
where μ_{0} is a constant that represents the chemical potential at a standard state, and γ is the activity coefficient which represents the effects of interactions among the atoms/molecules. For a dilute solution, interactions among the atoms/molecules are negligible; thus, γ = 1.
We focus on the stressdependent part of the chemical potential τ(E^{e}, C), which is the derivative of strain energy density W with respect to the concentration of lithium C. Traditionally, Π(X, t) is considered to be Helmholtz free energy density and therefore this step is carried out for fixed deformation written as [11]
The subscript H means that it is caused by the Helmholtz free energy density. The chemical potential turns out to be
where σ_{m} is the Cauchy hydrostatic stress in Eulerian description and can be obtained by
It is worth to note that the stiffness C of the electrode material is assumed to be independent of the concentration of lithium C in Eq. (12). In addition, det(F^{e}) ≈ 1 is widely accepted so that it is ignored usually. In the rest of this paper, we call Eq. (26) as the traditional expression of chemical potential. On the other hand, Π(X, t) is considered to be the Gibbs free energy density in some studies [12, 13] on phase field model so that we cannot get a developed expression of τ(E^{e}, C), and
The subscript G means that it is caused by the Gibbs free energy density. In this case, μbecomes
and we call Eq. (29) as the developed expression of chemical potential.
The mass transport equation is consisted by Eqs. (19), (20), (26), and (29) with traditional and developed expressions of chemical potential. In the remaining part of this paper, we will compare the effects of these two expressions of chemical potential on the diffusion induced stress and Li concentration under different charging methods.
In thermodynamics, the Helmholtz free energy is a thermodynamic potential that measures the useful work obtainable from a closed thermodynamic system at a constant temperature and volume. In contrast, the Gibbs free energy measures the maximum of reversible work that may be performed by a thermodynamic system at a constant temperature and pressure. In solids with low stress level, the Gibbs free energy is approximately equivalent to the Helmholtz free energy, because the deformation of solids is small usually. This assumption is suitable for most solid materials due to their small diffusion induced deformation, but except for silicon because of its large volumetric expansion during lithiation. In fact, diffusion and deformation take place at the same time, so that it is not suitable assuming that there is no deformation happening while the concentration is changing. Even so, as can be seen from Eq. (25), the traditional expression of chemical potential is still accurate when the deformation rate is low enough. However, it is likely to cause great errors when a Si nanoparticle electrode is lithiated rapidly.
The electrode is lithiated with a constant lithiumion concentration on its surface, namely the potentiostatic operation, or with a constant flux on its surface, namely the galvanostatic operation. The boundary conditions of Eq. (19) are
respectively. The initial condition is written as
for each charge operation. Here, C_{max} is the maximum lithium concentration of the material and j_{0} is a constant representing the charge current.
Numerical Implementation
It is very difficult to obtain the analytical solution of the above system consisting of partial differential equations, if not impossible. With Eqs. (1)–(3) and (13)–(18), we calculate the evolution of diffusioninduced stress and lithium concentration numerically by using the COMSOL multiphysics software. The lithiation of a silicon nanoelectrode under both potentiostatic and galvanostatic operations are studied, with different expressions of chemical potential. The material properties of Si and operating parameters used in the simulation are listed in Table 1. For convenience, the corresponding dimensionless substitution of coordinate, stress, and concentration are used in the figures.
To investigate the difference between the different expressions of chemical potential at different times in the spherical Si electrode, the state of charge (SOC) is calculated as
The stressinduced diffusion fluxes in the Lagrangian description are described as
representing the flux caused by different chemical potential expressions, respectively.
Results and Discussion
Figure 1 shows the spatial distribution of the concentration of lithium, radial stress, and hoop stress in a spherical Si electrode under galvanostatic operation at several SOCs. For comparison, the numerical results with both the developed and traditional expressions of chemical potential are included and they are represented by solid lines and triangles symbols, respectively. For each SOC in Fig. 1a, the solid line nearly overlaps the triangle symbols. The effect caused by the different expressions of chemical potential on the concentration of lithium can be ignored. In Fig. 1b and Fig. 1c, for the SOCs of 46.7% and 65.5%, the solid lines are higher than the triangles in the center, while they almost overlap outside, just like that at other SOCs. On the whole, there is a slight effect on the concentration of lithium and stresses under galvanostatic operation. Figure 2 shows the spatial distributions of the concentration of lithium, radial stress, and hoop stress in a spherical Si electrode under potentiostatic operation at several SOCs. It is worth mentioning that the radial and hoop stresses first increase and then decrease with the increase of SOC in both Fig. 1 and Fig. 2. It is because that the silicon electrode at the initial state or fully lithiated state is stressfree, since there is no concentration gradient. Compared with Fig. 1a, the difference between solid lines and triangles is greater in Fig. 2a. Due to the lithium concentration on the surface is a constant C_{max} under potentiostatic operation, the charge rate is higher than the deformation rate that of galvanostatic operation and the deformation rate as well. However, the total deformation under the same SOC is almost the same regardless of the charge method, just taking different time. It indicates that the influence on the distribution of lithium caused by different expressions of chemical potential is only related to the deformation rate rather than the deformation and increases with the increase of the deformation rate. In fact, existing experiments show that silicon electrodes deform very quickly during lithiation under certain charging modes. As we can see from Fig. 3 [17], the Si anode is fully deformed in 1 min with a 2V potential with respect to the Li metal. In this condition, the results solved by these two expressions of chemical potential will be significantly different. Unfortunately, in this case, the stress of the electrode cannot be measured accurately and therefore cannot be quantitatively compared with our model.
Figure 4 shows the spatial distribution of J_{H}/J_{G} in a spherical Si electrode at different SOCs under galvanostatic operation with different j. In Fig. 4, the solid lines almost coincide with the triangles, which indicates that different chemical potential expressions have a slight effect on the ratio of J_{H} and J_{G}. It is evident that the range of the values of J_{H}/J_{G} increases with the increase of the charge current. This is because the larger charge current leads to higher deformation rates and therefore causing the greater impact of different expressions of chemical potential. The ratio is always greater than 1 in the center and less than 1 on the surface. It suggests that the flux obtained from the developed expression of chemical potential on the surface is larger than that obtained from the traditional expression, while the opposite is true in the center. We notice that all the solid lines and triangles in Fig. 4 nearly intersect with one point. In addition, the ratio corresponding to the intersection is always about 1 no matter which current the electrode is charged with. It suggests that there is a critical radius where the flux is less affected by the different chemical potential expressions. We call it the chemical potential independent region (CIR). Obviously, CIR is always near the surface of the spherical electrode and is closer to the surface as the charge current increases.
By comparing the traditional and developed chemical potentials in Eq. (26) and Eq. (29), it is found that the Cauchy hydrostatic stress σ_{m} is the key to the difference between these two expressions. In order to investigate the causes of CIR, the spatial distribution of σ_{m}/E in a spherical Si electrode at different SOCs under galvanostatic operation with different expressions of chemical potential are given in Fig. 5 and Fig. 6. Obviously, nearly all curves intersect at one point in CIR and the Cauchy hydrostatic stress σ_{m} is close to 0 in this point, except at the beginning of charging (SOC = 6.2%). It indicates that σ_{m} in CIR is kept at a low level (nearly 0) for most of the charge period. It can be interpreted that the two chemical potential expressions are nearly equivalent when the hydrostatic stress σ_{m} is close to 0. This may partly explain why CIR appears, but it is not enough to explain the features of curves on σ_{m}. It needs to be solved by our next research.
Conclusions
In this work, a developed expression of chemical potential is proposed without the low deformation rate assumption, distinguished from the developed expression which is widely used at present. The difference between the traditional and developed expressions of chemical potential on the distributions of stress and concentration in Si nanoparticle electrodes is discussed under both potentiostatic and galvanostatic operations.
The result reveals that the effect caused by different expressions of chemical potential can be neglected under galvanostatic operation, but it is significant under potentiostatic operation. It is found that the effect is just related to the deformation rate rather than the deformation, and it can be greater with the increase of deformation rate. Considering the low deformation rate assumption in the traditional chemical potential expression, it is believed that the results obtained by the developed chemical potential expression are more reliable. A chemical potential independent region (CIR), where the flux caused by traditional and developed chemical potential is almost the same during most of the lithiated process, is found near the nanoparticle electrode surface. In addition, CIR is closer to the surface with the increases of charge current. A similar phenomenon also appears in the Cauchy hydrostatic stress curves. The Cauchy hydrostatic stress σ_{m} keeps a constant and maintained at a low level (nearly 0) in CIR at the most time, no matter which chemical potential expression is used. Such results have not yet been reported in the literature.
Availability of Data and Materials
The datasets analyzed during the current study are available from the corresponding author on reasonable request.
Abbreviations
 CIR:

A region where the diffusion flux caused by these two expressions of chemical potential is nearly same
References
Aricò AS, Bruce P, Scrosati B, Tarascon JM, Van Schalkwijk W (2005) Nanostructured materials for advanced energy conversion and storage devices. Nature Materials 4(5):366–377
Kasavajjula U, Wang C, Appleby AJ (2007) Nano and bulksiliconbased insertion electrodes for lithiumion secondary cells. J Power Sources 163(2):1003–1039
Shukla AK, Kumar TP (2008) Materials for nextgeneration lithium batteries. Current Science 94(3):314–331
Christensen J, Newman J (2006) Stress generation and fracture in lithium insertion materials. J Solid State Electrochem 10(5):293–319
Yang H, Fan F, Liang W, Guo X, Zhu T, Zhang S (2014) A chemomechanical model of lithiation in silicon. J Mechanics Physics Solids 70(1):349–361
Li Y, Zhang K, Zheng B, Yang F (2016) Effect of local velocity on diffusioninduced stress in largedeformation electrodes of lithiumion batteries. J Power Sources 319:168–177
Zhao K, Pharr M, Vlassak JJ, Suo Z (2011) Inelastic hosts as electrodes for highcapacity lithiumion batteries. J App Physics 109(1):31
Larché FC, Cahn JW (1985) The interactions of composition and stress in crystalline solids. Acta Metallurgica 33(3):331–357
Wu CH (2001) The role of Eshelby stress in compositiongenerated and stressassisted diffusion. J Mechanics Physics Solids 49(8):1771–1794
Cui Z, Gao F, Qu J (2012) A finite deformation stressdependent chemical potential and its applications to lithium ion batteries. J Mechanics Physics Solids 60(7):1280–1295
Gao YF, Cho M, Zhou M (2013) Stress relaxation through interdiffusion in amorphous lithium alloy electrodes. J Mechanics Physics Solids 61(2):579–596
Zuo P, Zhao YP (2016) Phase field modeling of lithium diffusion, finite deformation, stress evolution and crack propagation in lithium ion battery. Extreme Mechanics Letters 9:S2352431615300420
Deng J, Wagner GJ, Muller RP (2012) A phase field model of solid electrolyte interface formation in lithiumion batteries. Mrs Proceedings 1440(3):A487
Siladitya DAMLE, Sameer S, PATEL HS, DATTA KM, KUMTA NP (2014) Modeling the delamination of amorphoussilicon thin film electrode for lithiumion battery. J Power Sources 246(3):149–159
Zhao K, Pharr M, Cai S, Vlassak JJ, Suo Z (2011) Large plastic deformation in highcapacity lithiumion batteries caused by charge and discharge. J Am Ceramic Soc 94(s1):s226–s235
Peng YZ, Kai Z, Zheng BL, Yong L (2016) Stress analysis of a cylindrical compositiongradient electrode of lithiumion battery in generalized plane strain condition. Acta Physica Sinica 65(10)
Liu XH, Zhong L, Huang S, Mao SX, Zhu T, Huang JY (2012) Sizedependent fracture of silicon nanoparticles during lithiation. ACS Nano 6(2):1522–1531
Acknowledgements
Not applicable
Funding
The authors are grateful for the support from the Natural Science Foundation of China (No. 11672210).
Author information
Authors and Affiliations
Contributions
The numerical simulation was carried out by WF and ZK. WF was a major contributor in writing the manuscript, under the guidance of Z BL. All authors read and approved the final manuscript.
Corresponding authors
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Wang, F., Zhang, K. & Zheng, B. A developed expression of chemical potential for fast deformation in nanoparticle electrodes of lithiumion batteries. Nanoscale Res Lett 14, 262 (2019). https://doi.org/10.1186/s1167101930948
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/s1167101930948
Keywords
 Chemical potential
 Fast deformation
 Diffusioninduced stress
 Lithiumion batteries